Intermediate structures in two-dimensional molecular
1Nanoscale Materials Science, Empa, Swiss Federal Laboratories for Materials Testing and Research, Ueberlandstr. 129, CH-8600 D¨ubendorf, Switzerland
2Fachbereich Chemie, Universit¨at Z¨urich, CH-8057 Z¨urich, Switzerland E-mail: Karl-Heinz.Ernst@empa.ch
Received May 28, 2010; accepted June 20, 2010
We discuss the occurrence of transition structures observed in molecular self-assembly at surfaces. The increasing surface coverage transitions from low coverage structures to high coverage structures are a common phenomenon. However, often observed and not perfectly understood is the formation of intermediate structures, sometimes with lower lateral density than the initial phase. We will present diﬀerent examples from our recent work and discuss the possible mechanisms of intermediate phase formation. In addition, we present intermediate structures occurring due to temperature-controlled reversible phase transitions.
Keywords scanning tunnelling microscopy (STM), polymorphism, corannulene, heptahelicene,
PACS numbers 82.65.+r, 61.05.jd, 68.35.Ja, 61.43.-j, 64.75.Yz Contents
1 Introduction 340
2 Temperature-induced intermediate phases 340 2.1 Reversible 2-D phase transitions 341
2.1.1 A thermodynamically stable
2.1.2 A metastable phase via transition
2.2 A 2-D glass coexisting with ordered phases 342 3 Coverage-dependent intermediate phases 342
3.1 Azimuthal reorientation 342
3.1.1 Helical aromates 342
3.1.2 A bowl-shaped phthalocyanine 344
4 Conclusions 344
5 Methods and materials 345
Polymorphism, the phenomenon that a single com-pound can appear in diﬀerent crystal modiﬁcations, is of paramount importance in pharmaceutical and materi-als science. A new polymorph, for example, may act as contamination, inhibiting formation of other polymorphs in a laboratory forever . This has been experienced
with the anti-viral drug Ritonavir, which had to be with-drawn from the market after a new, less soluble crystal form appeared in a new synthesis batch . Polymorph control is therefore critical for the success of a pharma-ceutical product . The mechanism of how one poly-morph induces re-crystallization of another is not under-stood. Important steps include molecular stereochemi-cal recognition at the crystal surface and a solid-state phase transition . Solid–solid phase transitions and metastable polymorphs are common, making polymorph selection challenging. Nature teaches us, however, that control of polymorphism is possible, since many organ-isms “choose” shape, habit and polymorph of inorganic minerals in biomineralization .
It has been demonstrated that studies of well-deﬁned model systems help to unravel details of surface reac-tions . Consequently, the self-assembly of molecules on single crystal surfaces is increasingly deployed as an ap-proach for better understanding of stereochemical recog-nition at surfaces . In particular, scanning tunnelling microscopy (STM) allows monitoring these complicated processes at the molecular level .
Temperature-induced intermediate phasesFivefold-symmetry is regularly observed in nature and
chemistry, but is incompatible with the translational or-der of a classical crystal lattice . There are strong indications that supercooled liquids and metallic glasses possess icosahedral short-range order , and this geom-etry might be equally important for the glass transition and the structure of liquids during the melting process . But how does a liquid freeze if the geometry of its molecules prevents close packing into a regular crystal? Or how do such molecules arrange themselves on a sur-face when they adsorb from a solution or the gas phase? In order to realize a perfect tiling in a plane, ﬁvefold-symmetric shapes must be combined with other shapes [12, 13]. However, exclusive C5v symmetry cannot be maintained in a periodic tiling in two-dimensional (2-D) supramolecular structures .
2.1 Reversible 2-D phase transitions
2.1.1 A thermodynamically stable intermediate
We have studied the adsorption of corannulene (C20H10) on the copper (110) and (111) surfaces [15–19]. Coran-nulene (1, Fig. 1) is a curved, C5v-symmetric aromatic molecule with one pentagonal ring centred among hexag-onal rings, thus representing a segment of C60 buckmin-sterfullerene . At room temperature on Cu(111) a regular (4 0, 0 4)# array is observed for the complete corannulene monolayer (Fig. 1). Upon cooling, the 2-D crystal undergoes two diﬀerent phase transitions. At 225 K a denser (4 0, 3 7) lattice forms, followed by forma-tion of a (4 2, 0 7) structure with further decreasing perature. Each structure is stable in its respective tem-perature interval. This is conﬁrmed by the reversibility of the transitions (Fig. 1): When the low-temperature phase is heated, the medium-temperature phase forms again and is then converted completely into the (4 0, 0 4) phase at room temperature. To our knowledge, this is the ﬁrst observation of an enantiotropic phase transition in a 2-D organic molecular crystal. Both transitions show a hysteresis in temperature. The (4 0, 3 7) structure ex-ists at temperatures between 200 and 250 K. The highest temperature observed for the (4 2, 0 7) structure was 236 K upon cooling and 271 K while heating.
The molecules in all three structures are imaged asym-metrically. This indicates a substantial tilt of the molec-ular bowl with respect to the surface plane and agrees well with a geometry in which the molecules are oriented with one of the ﬁve C6 rings parallel to the surface. Den-sity functional theory (DFT) actually predicts the hexag-onal ring to be located above a threefold hollow site . For the (4 0, 3 7) intermediate structure, however, the two molecules of the unit cell are located
Fig. 1 Scheme of two reversible phase transitions between three polymorphs of 1 on Cu(111). STM images of the three observed phases (averaged from 186, 64, and 17 diﬀerent positions, respec-tively). The unit cells and the molecular azimuthal orientations are indicated (scale bars are 1 nm). A ball-and-stick model of 1, the unit cells on the copper grid and the matrices are also given. The intermediate (4 0, 3 7) phase is only observed between 200 K and 250 K.
on diﬀerent sites, i.e., one on an fcc threefold hollow site, the other on a hcp threefold hollow site. The longer unit cell vector runs at a small oblique angle with respect to the 1 1 ¯2 substrate directions (Fig. 1). Hence, the structure is enantiomorphous, i.e., reﬂection symmetry is broken and mirror-domains exist. Rotational domain boundaries therefore show a tilt angle for molecular rows as well (Fig. 2, inset). The two lower temperature phases are substantially denser (1.26 molecules/nm2) than the room temperature phase (1.10 molecules/nm2), so the lattice density changes substantially during the (4 0, 0 4)/(4 0, 3 7) transition, but not for the (4 0, 3 7) to (4 2, 0 7) transition. Without changing the number of molecules on the surface, the lattice density is increased by 14.5% during the ﬁrst transition.
Fig. 2 STM image of the intermediate phase meta-stabilized at 67 K [10 nm× 10 nm, averaged over 59 positions (–2 V, 1 nA)]. The inset (10 nm× 10 nm) shows a rotational domain boundary.
Attractive intermolecular interactions clearly drive the ﬁrst transition upon cooling and increase the binding en-#The two-by-two transformation matrix (m11 m12, m21 m22) links the adsorbate lattice vectors (b1, b2) to the substrate lattice
thalpy. Hence, the (4 0, 0 4) phase must have higher en-tropy due to vibrational excitations . That excitation of vibrations at higher temperature lead to occupation of more space is well accepted and has been demonstrated recently for benzene . Depopulation of vibrational states by means of cooling decreases the spatial require-ments of the molecules and allows closer packing.
2.1.2 A metastable phase via transition blocking
The intermediate phase could be stabilized by soft breathing modes of the buckybowl as well. The driv-ing force for the low-temperature (LT) phase transition upon cooling, however, is presumably the occupation of identical threefold hollow substrate sites in the LT phase, which are energetically slightly favoured. Although both phases have identical density, more space is needed dur-ing the transition. By lateral conﬁnement with addi-tional molecules, we succeeded to block this transition . In that case the (4 0, 3 7) intermediate phase was stabilized down to 60 K, a metastable structure at that temperature. This allowed, in turn, to achieve better resolved STM images (Fig. 2).
2.2 A 2-D glass coexisting with ordered phases
As a consequence of the contraction upon cooling, the bare copper surface must be revealed in other areas. Sin-gle molecules, too mobile to be imaged in STM, form a 2-D gas in these areas, but further cooling leads to 2-D solidiﬁcation. Figure 3 shows STM images of the re-sult. In part, no long-range order is observed and a 2-D glass of low density has been formed. Upon solidiﬁca-tion of the 2-D gas, we also observe density ﬂuctuasolidiﬁca-tions and locally mid-range ordering with higher density. That is, patches of ordered structures surrounded by the 2-D glass. Figure 3a shows such a new ordered phase embed-ded in the glassy area. This perfectly periodic structure contains diﬀerent types of molecular orientations. Molec-ular bowls pointing upright are arranged into trimers (C3 symmetry), which are lined-up in rows. These rows are decorated with tilted molecules at the gaps between the trimers. In addition, located between these rows are ziczac rows of tilted molecules. Overall, there are seven molecules in this large unit cell. In areas with even higher density in the glass phase, structures with all molecules tilted into the same direction are observed again. Fig-ure 3(b) shows an STM image of such ordered structFig-ure. Quite surprisingly, the lattice is almost quadratic, which is compatible with the underlying hexagonal metal sub-strate only in a (4 3, –1 3) lattice. This shows that at low temperature (74 K) the locally self-assembled lat-tice due to solidiﬁcation is slightly denser (equivalent to 15 Cu atoms) than the (4 × 4) lattice (16 Cu atoms), which is observed at room temperature for the saturated
Fig. 3 (a) STM image (50 nm× 50 nm) of an area showing an
ordered structure within the glass. The inset shows an averaged seven-nm-image [parameters: –2000 mV, 200 pA, 1149 nm/s, 72 K, (inset) is averaged over 17 positions]. (b) STM image (50 nm× 50 nm) of a rectangular structure with medium density. Domains of this structure are marked yellow. The analysis shows a (3 4, –3 1) matrix and hence a local coverage of 1/15 molecules per Cu atom. The blue lines mark the denser LT phase (parameters: –1800 mV, 50 pA, 781 nm/s, 66 K).
Formation of these structures is explained by diﬀu-sion kinetics. At the low density of the 2-D gas, these low-density structures nucleate, but they are not able to grow further due to the limited diﬀusion with falling temperature. For the same reason, the LT phase does not completely dominate at low temperatures and the 2-D glass appears.
Coverage-dependent intermediate phases3.1 Azimuthal reorientation
3.1.1 Helical aromates
2-D crystallization of the chiral aromatic hydrocarbon heptahelicene [Fig. 4(a) top, C30H18, [7 ] H] on metal surfaces is an exciting chapter of surface chirality. While on nickel surfaces no extended ordering phenomena has been found [24–26], a pronounced transfer of chirality into mono-and multilayered structures, manifested by the formation of extended chiral motifs, was observed for the pure enantiomers on Cu(111) [27, 28]. Interestingly, mirror domains have been observed for the racemate at the same surface, indicating at a ﬁrst glance a lateral resolution of the enantiomers . However, STM ex-periments in combination with molecular modeling cal-culations (MMC) showed that heterochiral M–P pairs become aligned in a chiral zigzag conﬁguration (Fig. 4), leading to the observed enantiomorphism . A switch to the opposite enantiomorph requires only a small re-arrangement of the enantiomers in the heterochiral pair. This leads to the induction of lattice homochirality via cooperative ampliﬁcation of a small chiral bias in non-racemic mixtures . This kind of ampliﬁcation of chirality is quite similar to the “sergeants-and-soldiers”
principle, ﬁrst reported for helical polymers with chiral side chains in solution . In two dimensions this phe-nomenon has been ﬁrst observed by us for racemic mono-layers of prochiral succinic and meso-tartaric acid after doping with intrinsically chiral (R,R)-or (S,S)-tartaric acid [32–34]. The corresponding ampliﬁcation of chiral-ity in helical copolymers with small enantiomeric excess in the side chains has been coined as “majority rule” , and the 2-D analogue has been reported recently .
Fig. 4 Helicene polymorphs. (a) Top: Ball-and-stick model of the two [7 ] H enantiomers. Bottom: STM image of [7 ] H phases at medium coverage. Theλ/ρ phase (only theρenantiomorph is shown) is an intermediate between the ε/δ phase and the λ/ρ phase at saturation coverage (b). At lower coverage only the do-mains of theε/δ phase are observed. The insets show the zigzag motif for theδ structure [(a) Bottom] and for the ρ tructure (b).
No ordered superstructures are observed up to cov-erages close to half a monolayer. Even at 50 K, single molecules are too mobile to be imaged via STM on the ﬂat Cu(111) terraces. Hence, the diﬀusion barrier for the individual molecule is either low enough to allow the molecules to diﬀuse to the step edges where they get pinned, or they are moved by the STM tip. The molecules are only observed to decorate the lower part of step edges, forming one-dimensional chains. Since the [7 ] H molecules exhibit no chemical groups to form stronger directional intermolecular bonds, they do not coalesce into 2-D islands at small coverage and are imaged as unstable patterns by the STM. This mobile phase (2-D gas) starts to condensate at about 50% of the sat-urated monolayer coverage, and short chains of [7 ] H molecules appear to nucleate randomly over the terraces. With increasing coverage enantiomorphous lattice struc-tures embedded in areas of short-ranged ordered fea-tures are observed. Figure 4 presents STM images for the racemate at medium coverage and saturation. Over-all, three pairs of enantiomorphous structures, denoted as ε/δ, λ/ρ and λ/ρ, are observed . All these ad-lattices successively form with increasing global cover-age and have a common feature, i.e., the molecules are aligned in zigzag double rows (see insets of Fig. 4).
The structural diﬀerence between the zigzag rows of theε/δ and the λ/ρ phase is, besides the slight diﬀerence
in coverage (0.93 molec./nm2and 0.96 molec./nm2), the relative azimuthal alignment of the helices in the double rows plus the alignment of the rows relative to the sub-strate. Figure 5 shows the models for both structures. For theε/δ structure the intermolecular distances within a double row are smaller, but the distance between rows is larger.
Fig. 5 (a), (b) Model for the δ domain and the λ domain.
Molecules are presented by disks. The arrows and the bright oﬀ-centre protrusions mark the overlap between the terminal rings of [7 ] H. (c) STM image of a phase boundary between the in-termediate structure ρ and the saturation structureρ. Except the inter-double row distance, all other structural parameters are identical. (d) Phase diagram for the racemate with increasing
coverage and for unequal mixtures (e.e. = 0) of the enantiomers. Small enantiomeric excess (e.e.) lets only one enantiomorph exist.
Both phases are closely packed and it comes as a sur-prise that the intermediate phase that appears with in-creasing global coverage after theε/δ phase, has a much lower density (0.77 molec./nm2). The azimuthal align-ment, however, is identical with theλ/ρ structure. Only the inter-row distance is substantially larger [Fig. 5(c)]. In order to form the densest and most stableλ/ρ pack-ing at saturation coverage, the transition from the dense
ε/δ phase goes through the loosely packed – but with
re-spect to the ﬁnal phase equally aligned –λ/ρphase. We must keep in mind here that only certain adsorbate sites provided by the substrate crystal and certain azimuthal orientations due to the steric interaction between the he-lices are allowed. This explains the more or less abrupt switch in orientation in the transition fromε/δ to λ/ρ. With increasing lateral pressure the relative azimuthal alignment of the molecules in theε/δ phase apparently becomes destabilized. This leads to the (counterintu-itive) situation that locally a less favored structure is formed [Fig. 4(a) Bottom], while globally the energy of
the system decreases due to minimizing lateral pressure. This allows maintaining the dense ε/δ phase as part of the monolayer. The λ/ρ phase is truly an intermedi-ate structure. It can only coexist together with theε/δ phase. With further increasing coverage the ε/δ phase disappears, while the λ/ρ phase converts step-by-step intoλ/ρ domains [Fig. 5(d)]. A phase diagram including the structures for the pure enantiomers can be found in Ref. .
3.1.2 A bowl-shaped phthalocyanine
2-D crystallization of the subphthalocyanine (SubPc, Fig. 6, insets) reveals also interesting intermediate phases. SubPc is a special member in the family of metal-lic phthalocyanines because of its bowl geometry. It has only three isoindolyl groups instead of four in the com-mon MPc. The central boron atom is sp3-coordinated to all isoindolyl groups and to the axial chlorine atom, which leads to a bowl-shaped molecular frame. SubPc is still the only known threefold symmetric phthalocya-nine. SubPc adsorption and growth has been studied previously [38–42], whereby on Ag(111) SubPc was found to adsorb with the bowl opening pointing away from the surface. On Au(111) Jiang et al. recently reported an in-termediate phase that, similar to the [7 ] H/Cu(111) case, shows the coexistence of diﬀerently azimuthal-aligned structures. Figure 6 shows the observed structures for SubPC .
Fig. 6 STM images of diﬀerent phases of subPC on Au (111) with increasing global coverage (θ). (a) θ = 0.2, 25 nm ×25 nm,
U = −2.0 V, I = 60 pA. (b) θ = 0.6, 16 nm ×16 nm, U = −2.0 V, I = 100 pA. (c) θ = 0.6, 16 nm ×16 nm, U = −2.0 V, I =
100 pA. (d)θ = 1.0, 5 nm ×5 nm. The insets show the relative alignment of the molecules in the structures.
Depending on coverage and deposition temperature, four diﬀerent complex structures have been observed at 77 K in STM. The threefold symmetric molecule
ap-pears accordingly in the STM, i.e. as three-spoke entity. The initial (6 –3, 3 9) phase [Fig. 6(a), 0.032 molecules per Au atom] shows a wheel-network structure with the isoindolyl groups clockwise or counterclockwise geared to each other. As a consequence, mirror domains are found at the surface [Fig. 6(a)]. Attractive interactions domi-nate this structure, since island formation is observed. At higher global coverage, two coexisting phases are observed. One of the structures has identical local den-sity as the initial (6 –3, 3 9) structure, but there is no gearing in this “diamond” (6 –3, 3 9) phase . The relative orientation between adjacent molecules in the superlattice has changed such that the phenylene parts of two isoindolyl groups face each other [Fig. 6(b)].
The other “intermediate” structure is slightly higher in density and combines both structural features: the set-oﬀ observed for the initial phase plus the opposing pheny-lene rings of the diamond structure. In matrix notation the unit cell is characterized as (13 0, 0 13) with six molecules per unit cell (0.036 molecules per Au atom) In contrast to the corannulene case no temperature change is involved between the equally dense phases, but there is an increase in global density. When the diamond struc-ture nucleates and grows there are substantially more molecules on a single substrate terrace than in the case of the honeycomb formation. A limit in mobility could therefore impose a kinetic barrier, not allowing the ﬁnal reorientation into a honeycomb pattern. However, like in the [7 ] H case, another coexisting phase with diﬀerent density is present on the surface, but this time on diﬀer-ent terraces only. Nucleation and growth of the (more stable) denser phase leads to a subcritical coverage on other terraces. Upon further cooling, the diamond phase nucleates on the other terraces with coverages below the critical value needed for intermediate phase nucleation. This mechanism is further supported by the fact that many “diamond” domains exist on a single terrace. The boundaries cannot disappear and heal, because the tem-perature became too low. In that respect, “diamond” and “intermediate” must coexist and both structures are actually metastable transitional phases between the low-coverage honeycomb (ruled by attraction forces) and the saturation coverage (4 –1, 1 5) phase that forms only upon annealing during deposition (0.048 molecules per Au atom).
Increasing global coverage leads to coexisting intermedi-ate phases during nucleation and 2-D growth, which not necessarily have higher coverage than the initial phases. Our examples include diﬀerent equal local density or even lower local density phases, which are in compe-tition with other more stable phases during nucleation
and growth. Falling temperature kinetic barriers due to lower mobility induces critical phenomena, not leading to the structure that would form without competition. Such situation is also induced by temperature-induced phase transitions with local density change. The limited mobility leads to 2-D glass and patches of low-density ordered structures. Finally, an intermediate phase that is thermodynamically stable in the temperature range between 200 K and 250 K was (meta) stabilized due to conﬁnement with other molecules down to 60 K. These examples show that high-resolution methods, like STM, are very valuable in order to study nucleation, growth and polymorphism, phenomena that are tremendously important for the three-dimensional outcome of materi-als systems.
Methods and materials
The adsorbate system has been investigated under ultra-high vacuum (UHV) conditions (p ≈ 10−8 Pa). Coran-nulene, heptahelicene and subPC have been evaporated from eﬀusion cells in vacuo onto the copper and gold crystals at room temperature. The crystal surfaces have been cleaned via standard sputtering and annealing cy-cles as described in detail before [44–46]. Cleanliness and quality of the surfaces and the surface coverage of the adsorbate systems have been determined with STM. Corannulene of high purity was prepared by literature methods . Synthesis and enantiomeric separation (e.e. > 99.9 %) of heptahelicene ( H) has been per-formed as described previously [29, 48]. The absolute conﬁguration was assigned with a high level of conﬁ-dence by comparison of experimental and calculated VCD spectra . X-ray photoelectron diﬀraction stud-ies (XPD) of (M)- H on the stepped Cu(332) surface conﬁrmed this assignment .
Acknowledgements Support by the Schweizerischer National-fonds was gratefully acknowledged.
1. J. D. Dunitz and J. Bernstein, Acc. Chem. Res., 1995, 28: 193
2. J. Bauer, S. Spanton, R. Henry, J. Quick, W. Dziki, W. Porter, and J. Morris, Pharm. Res., 2001, 18: 859 3. R. Hilﬁker (Ed.), Polymorphism in the Pharmaceutical
In-dustry, Weinheim: Wiley-VCH, 2006
4. I. Weissbuch, L. Addadi, M. Lahav, and L. Leiserowitz, Sci-ence 1991, 253: 637
5. L. Addadi and S. Weiner, Proc. Natl. Acad. Sci., 1985, 82: 4110
6. G. Ertl, Angew. Chem. Int. Ed., 2008, 47: 3524 7. K.-H. Ernst, Top. Curr. Chem., 2006, 265: 209
8. S. De Feyter and F. De Schryver, Chem. Soc. Rev., 2003, 32: 139
9. M. J. Buerger, Elementary Crystallography: An Introduc-tion to the Fundamental Geometrical Features of Crystals, New York: Wiley, 1956
10. D. Shechtmann, I. Blech, D. Cratias, and J. W. Cahn, Phys. Rev. Lett., 1984, 53: 1951
11. D. R. Nelson, Phys. Rev. B, 1983, 28: 5515
12. I. Hargittai (Ed.), Fivefold Symmetry, Singapore: World Scientiﬁc, 1992
13. R. L¨uck, Mater. Sci. Eng. A, 2000, 294–296: 263
14. K. E. Plass, A. L. Grzesiak, and A. J. Matzger, Acc. Chem. Res., 2007, 40: 287
15. T. Bauert, L. Merz, D. Bandera, M. Parschau, J. S. Siegel, and K.-H. Ernst, J. Am. Chem. Soc., 2009, 131: 3460 16. M. Parschau, R. Fasel, K.-H. Ernst, O. Gr¨oning, L.
Bran-denberger, R. Schillinger, T. Greber, A. P. Seitsonen, Y. T. Wu, and J. S. Siegel, Angew. Chem. Int. Ed., 2007, 46: 8258
17. L. Merz, M. Parschau, L. Zoppi, K. K. Baldridge, J. S. Siegel, and K.-H. Ernst, Angew. Chem. Int. Ed., 2009, 48: 1966
18. L. Merz, T. Bauert, M. Parschau, G. Koller, J. S. Siegel, and K.-H. Ernst, Chem. Commun., 2009: 5871
19. L. Merz, M. Parschau, J. S. Siegel, and K.-H. Ernst, Chimia, 2009, 63: 214
20. Y. T. Wu and J. S. Siegel, Chem. Rev., 2006, 106: 4843 21. A. I. Kitajgorodskij, Acta. Cryst., 1965, 18: 585
22. J. D. Dunitz and R. M. Ibberson, Angew. Chem. Int. Ed., 2008, 47 4208
23. L. Merz and K.-H. Ernst, Surface Sci., 2010, 604: 1049 24. K.-H. Ernst, M. B¨ohringer, C. F. McFadden, P. Hug, U.
M¨uller, and U. Ellerbeck, Nanotechnology, 1999, 10: 355 25. K.-H. Ernst, M. Neuber, M. Grunze, and U. Ellerbeck, J.
Am. Chem. Soc., 2001, 123: 493
26. K.-H. Ernst, Y. Kuster, R. Fasel, C. F. McFadden, and U. Ellerbeck, Surf. Sci., 2003, 530: 195
27. R. Fasel, M. Parschau, and K.-H. Ernst, Angew. Chem. Int. Ed., 2003, 42: 5178
28. M. Parschau, U. Ellerbeck, and K.-H. Ernst, Colloids and Surfaces A: Physicochem. Eng. Aspects, 2010, 354: 240 29. K.-H. Ernst, Y. Kuster, R. Fasel, M. M¨uller, and U.
Eller-beck, Chirality, 2001, 13: 675
30. R. Fasel, M. Parschau, and K.-H. Ernst, Nature, 2006, 439: 449
31. M. M. Green, M. P. Reidy, R. J. Johnson, G. Darling, D. J. O’Leary, and G. Wilson, J. Am. Chem. Soc., 1989, 111: 6452
32. M. Parschau, S. Romer, and K.-H. Ernst, J. Am. Chem. Soc., 2004, 124: 15398
33. M. Parschau, T. Kampen, and K.-H. Ernst, Chem. Phys. Lett., 2005, 407: 433
34. K.-H. Ernst, Curr. Opin. Colloid Interface Sci., 2007, 13: 54
35. M. M. Green, B. A. Garetz, B Munoz, H. Chang, S. Hoke, and R. G. Cooks, J. Am. Chem. Soc., 1995, 117: 4181 36. S. Haq, N. Liu, V. Humblot, A. P. J. Jansen, and R. Raval,
37. M. Parschau, R. Fasel, and K.-H. Ernst, Cryst. Growth & Des., 2008, 8: 1890
38. H. Yanagi, D. Schlettwein, H. Nakayama, and T. Nishino, Phys. Rev. B, 2000, 61: 1959
39. S. Berner, M. Brunner, L. Ramoino, H. Suzuki, H.-J. G¨untherodt, and T. A. Jung, Chem. Phys. Lett., 2001, 348: 175
40. S. Berner, M. de Wild, L. Ramoino, S. Ivan, A. Baratoﬀ, H.-J. G¨untherodt, H. Suzuki, and T. A. Jung, Phys. Rev. B, 2003, 68: 115410
41. H. Yanagi, K. Ikuta, H. Mukai, and T. Shibutani, Nano Lett., 2002, 2: 951
42. S. Mannsfeld, H. Reichhard, and T. Fritz, Surf. Sci., 2003, 525: 215
43. N. Jiang, Y. Wang, Q. Liu, Y. Zhang, K.-H. Ernst, and H.
J. Gao, Phys. Chem. Chem. Phys., 2010, 12: 1318 44. K.-H. Ernst, D. Schlatterbeck, and K. Christmann, Phys.
Chem. Chem. Phys. 1999, 1: 4105
45. B. Behzadi, D. Ferri, A. Baiker, and K.-H. Ernst, Appl. Surf. Sci., 2007, 253: 3480
46. M. Parschau, B. Behzadi, S. Romer, and K.-H. Ernst, Surf. Interface Anal., 2006, 38: 1607
47. T. J. Seiders, E. L. Elliott, G. H. Grube, and J. S. Siegel, J. Am. Chem. Soc., 1999, 121: 7804
48. A. Sudharkar and T. J. Katz, Tetrahedron Lett., 1986, 27: 2231
49. T. B¨urgi, A. Urakawa, B. Behzadi, K.-H. Ernst, and A. Baiker, New J. Chem., 2004, 28: 332
50. R. Fasel, A. Cossy, K.-H. Ernst, F. Baumberger, T. Greber, and J. Osterwalder, J. Chem. Phys., 2001, 115: 1020